Body bloating (larger bubbles) and blistering (smaller ones) occurs after a clay body matures to the point that the surface seals due to glass development but before generation of gases from decomposition of organic, carbonate or sulfate materials has completed. The internal pressures bubble the clay (since it has softened to the point of being flexible).
Some bodies cannot be fired to even near zero porosity
Bloating in an over fired middle temperature high iron raw clay (Plainsman M2). It is still stable, dense and apparently strong at cone 4 (having 1.1% porosity). But between cone 6 and 7 (top bar) it is already bloating badly. Such clays must be fired at low enough temperatures to avoid this volatility (if accidentally over fired). This clay only reaches a minimum of 1% porosity (between cone 4 and 5), it is not possible to fire it to zero porosity. This is because of the particulate gas-producing particles (it is ground to 42 mesh only).
What happens when you fired a terra cotta at cone 5-8?
This one can take more temperature than most. It looks OK at cone 5 (bottom bar). But at cone 6 bloating (bubbles) begin to occur. This body, while smooth to the touch, contains some iron and sulphate particulates that generate gases during firing, these are the catalyst for the bloating (the clay matrix becomes dense enough that it can no longer vent the gases of decomposition through it).
Iron oxide goes crazy in reduction
Cone 6 iron bodies that fire non-vitreous and burn tan or brown in oxidation can easily go dark or vitreous chocolate brown (or even melting and bloated in reduction). On the right is Plainsman M350, a body that fires light tan in oxidation, notice how it burns deep brown in reduction at the same temperature. This occurs because the iron converts to a flux and the glass development that occurs brings out the dark color. On the left is Plainsman M2, a raw high iron clay that is quite vitreous in oxidation, but in reduction it is bloating badly. When reduction bodies are this vitreous there is a much great danger of black coring.
What often happens when already vitrified ware is refired?
Bloating. These teapots have been refired to cone 6.
A cone 6 stoneware with 0.3% 60/80 mesh manganese granular (Plainsman M340). Fired from cone 4 (bottom) to cone 8 (top). It is normally stable to cone 8, with the manganese it begins to bloat at cone 7.
The best firing temperature for this body?
This cone 6 brown functional stoneware has been fired across a range of temperatures. Cone 4 is too porous. From cone 7 it is expanding and density is not improving, it will likely warp or bloat. Cone 7 is losing the red color, there is no room for over-firing (by accident). The porosity at cone 6 is so much better than cone 5 and color is still stable. Therefore, cone 6 is the one we want.
Why is the clay blistering on this figurine?
This is an admirable first effort by a budding artist. They used a built-in cone 6 program on an electronic controller equipped electric kiln. But it is over fired. How do we know that? To the right are fired test bars of this clay, they go from cone 4 (top) to cone 8 (bottom). The data sheet of this clay says do not fire over cone 6. Why? Notice the cone 7 bar has turned to a solid grey and started blistering and the cone 8 one is blistering much more. That cone 8 bar is the same color as the figurine (although the colors do not match on the photo). The solution: Put a large cone 6 in the kiln and program the schedule manually so you can compensate the top temperature with what the cone tells you.
Out Bound Links
In Bound Links